|Features:||Good Weather Resistance||Solid Content:||≥ 60%|
|Drying Time:||≤ 60 Min||Film Hardness:||2H|
|Hard Dry:||24h||Applicaton:||Flooring Coating|
Fast Drying Polyaspartic Flooring Coating,
Elastomer Topcoat Polyaspartic Flooring Coating
PH9502 High Weathering Resistance Polyaspartic Polyurea Floor Topcoats
PH9502 Polyaspartic polyurea flooring topcoats is a polyurea elastomer topcoat developed by Zhuhai Feiyang Novel Materials Corporation Limited, which applies explicitly to outdoor floor high weathering, scratch resistant rigid coating. It can be used directly on the Epoxy Floor to improve the floor weathering and scratch resistance performance. Its main components are aliphatic two-component poly aspartic acid ester polyurea. CIts main components are aliphatic two-component poly aspartic acid ester polyurea.
★ has fast drying, strong adhesion, wear resistance, and resistance to scratching performance, excellent resistance to yellowing.
★ decorative properties, can be made into various colors, coating fullness read good
★ acid performance
★ good weather resistance, resistance QUV accelerated aging test of 1200 hours. Long-term outdoor use.
★ convenient construction, can take a brush, roller, airless spray, and Conventional air spray in various ways.
★ For underground parking floor coating, top coat paint to improve floor scratch-resistant performance;
★ For various outdoor floor coating topcoats to replace fluorocarbon coating, weather-resistant polyurethane coating to improve the performance of ground resistance yellowing, scratch resistant;
★Used for a variety of exhibition halls, hotel lobbies, and other high-grade floor areas, improving coating scratch resistance, gloss, leveling, and fullness;
★Used in hospitals, hotels, exhibition halls, other interior and exterior decorative hanging plates, and other fields to improve the coating yellowing resistance, scratch resistance, and other properties.
Main performance indicators
Performance indicators technical indicators of the test items
Solid content (%) ≥ 60%
The fine degrees (μm) ≤ 25
Drying time dry ≤ 60 min
Hard work 24h (25 ℃ ± 2)
Film hardness 2H
Impact strength kg.cm 50 (positive and negative)
Taper wearable (500g/500r) almost no weight loss
Flexibility at low temperature ≤ -35 ℃, no cracks
Acid (0.1N sulfuric acid, 240h) No abnormality
Alkali resistance (0.1N sodium hydroxide, 240h) No abnormality
Resistant artificial climate accelerated test 1200h no obvious discoloration and chalking coating, no blistering, no cracks
Use poly urea topcoat: curing agent: thinner = 100:50: Moderate
Spray, brush, roller coating, airless spray
Construction period: 1.5h
Recoat: 10h (0.2mm) (depending on the temperature of the construction site and construction thickness maybe)
Store in a cool, dry, well-ventilated place, Do not expose dampness.
Be sure to mix agitation evenly and filter through a 200-mesh strainer.
The packaging specifications paint 20kg, 5kg;
Curing agent 10 kg, 1 kg
Storage and Transportation
The strains of flammable and explosive dangerous chemicals should be kept away from heat sources and cut off from the start of the fire to avoid severe impacts.
◇ construction, the two components are mixed and stirred evenly.
◇ unused paint should be kept under seal.
◇ construction should ensure good ventilation.
◇ This manual is a test, the accumulation of experience, and detailed construction details required by the construction design implementation.
Contact Person: Annie Qing
Tel: +86 18307556691